**2 **

### Original

### The long-wavelength-limit of structure factor and chemical

### ordering in binary Ag-In melts

### Raghvendu Pathak

*Department of Chemistry, Pachhunga University College, Aizawl 796001, India *

Received 7 September 2014 | Revised 25 January 2015 | Accepted 29 January 2015

**A**

**BSTRACT**

The long-wavelength-limit partial structure factors, Sxy(0), have been determined for liquid silver-indium (Ag-In) alloys using square well potential as perturbation over Percus-Yevick (PY) hard sphere reference system. Obtained Sxy(0) at various compositions of In have been employed to calculate isothermal compressibility and chemical ordering in the alloys. Further, homo-coordination and hetero-homo-coordination in Ag-In alloys have been studied at microscopic level in terms of mutual and intrinsic diffusion coefficients

Key words: Liquid alloys; structure factor; square well potential; diffusion coefficient.

*Corresponding author: *Pathak
Phone: +91-9436370190
E-mail: rppuc41@yahoo.com

**I**

**NTRODUCTION**

The microscopic structural, thermodynamic
and dynamic properties of binary liquid alloys
have been studied and of longstanding interest.
These studies are also important from
metallur-gical point of view.1_{ In recent years, many }

inves-tigations regarding compound forming behavior
and various thermodynamic properties as a
func-tion of concentrafunc-tion in binary liquid alloys from
their long-wavelength-limit of structure factors
have been reported, which are of importance
from scientific and technological points of view.2
-10_{ }

A good number of experimental, theoretical
and simulation results on structure, dynamic
and thermodynamic properties of Ag-In melts
11-15_{ are available in literature but knowledge about }

the chemical ordering in this alloy is desired. The complete structural characteristics in binary melts in momentum space can be described by three partial pair correlation functions (partial structure factors, PSFs) namely Sx-x(k), Sy-y(k)

and Sx-y(k). From these PSFs partial gxy(r) and

total g(r) radial distribution functions can be ob-tained. Partial Yxy and total Y coordination

number can by integrating gxy(r) and g(r)

func-tions in between first two minimum values of
these functions.16_{ }

In present paper, the direct correlation
func-tions (DCFs) of liquid Ag-In alloys were
deter-mined using Lebowitz solution17 _{of }

*Percus-Science Vision *15(1), 2-7

2015 January-March ISSN (print) 0975-6175 ISSN (online) 2229-6026

### Research

**3 **

Yevick (PY) equation for hard sphere model with square well attractive tail in limit of zero wave vector. From the DCFs long-wavelength- limit of PSFs SAg-Ag(0), SIn-In(0) and SAg-In(0) are

evaluated. The total structure factor in long-wavelength limit S(0), isothermal compressibil-ity KT, Bhatia-Thornton (BT) concentration –

concentration correlation function, in long-wavelength-limit SCC(0) were compute from long

- wavelength-limit of PSFs. The ratio of mutual diffusion coefficients (DM) and inter-diffusion

coefficients (Did) of components and chemical

short range order parameter (CSRO), α are also presented in the later part of this paper.

**T**

**HEORETICAL**

**FORMALISM**

Within the mean spherical model approximation (MSMA) the direct correlation functions (DCFs) in repulsive and attractive region of potential function can be given as 16

Cxy r = Cxy0 (r) − εxy

KBT (1)

where 𝐶𝑥𝑦0 (𝑟) is the DCF in the hard sphere region,

### 0

###

### r

###

### σ

_{xy}, obtained by Lebowitz 17 for Percus-Yevick equation, −

_{𝐾}𝜀𝑥𝑦

𝐵𝑇 is the direct correlation function (DCF) in the square well attractive region,

### σ

_{xy}

###

### r

###

### λ

_{xy}

### σ

_{xy}. The DCF beyond square well region is considered as 0 it means that there is no correlation between liquid atoms in the region

### r

###

### λ

_{xy}

### σ

_{xy}.

Further r is the separation between pair of atoms whereas xx, xx, and xx (xx-1) are the

diameter, the potential energy depth and
breadth respectively of the square well potential
of the xth_{ species. The mixed parameters are }

determined through the use of Lorentz Berthelot
rules 16_{. Thus, the mixed parameters are given }

by

###

###

###

###

###

###

###

###

###

###

###

###

###

12 2 22 1 11 12 1/2 22 11 12 2 1 12### σ

### 2

### σ

### λ

### σ

### λ

### λ

### )

### ε

### (ε

### ε

### 2

### /

### )

### σ

### (σ

### σ

(2)The Fourier transform of direct correlation
functions (DCFs) have been well explained
already 16_{ and will not be repeated here. }

However, in thermodynamic limit when k 0, DCFs can be given as

3

1 1 1 1

1 11 1

3 1 11 11

B

### a

### b σ

### dσ

### ρ C (0) 24 η

### 3

### 4

### 6

### 8 η ε (λ - 1)

### k T

###

###

###

_{}

###

###

_{}

###

###

###

(3) 32 2 2 2

2 22 2

3 2 22 22

B

### a

### b σ

### dσ

### ρ C (0)

### 24 η

### 3

### 4

### 6

### 8 η ε (λ - 1)

### k T

###

###

###

_{}

###

###

_{}

###

###

###

(4) 3 312 12 12 12

B 3 1 12

3 1 2

1

1 1 2

### 4π ε σ (λ - 1)

### C (0)

### 3 k T

### 4 π a σ

### -

### 3

### b (σ

### 2 σ )

### 4π σ {

### 12

### λ d σ (3σ 5 σ )

### +

### 10

###

###

###

###

21 1 2

### d σ (2σ

### 3 σ )

### +

### }

### 30

###

(5)
Here 1 stands for Ag (silver) and 2 for In
(indium), rest of the symbols used in equations 3
to 5 have been already explained elsewhere 19_{. }

Kirkwood and Buff 19_{ related the isothermal }

compressibility, KT of the mixture to x Cxx(0)

and 12 C12(0) as follows

B T 1 1 11 2 2 22

1 2 12 12

### ρ k T χ

### [1 - c ρ C (0) - c ρ C (0)

### - 2 c c ρ C (0)]

###

(6)

Here ρx is the number density of pure component and 12 = (12)1/2.

Three partial structure factors (PSFs) in the long-wavelength-limits can be written in terms of direct correlation functions C11(0), C22(0) and

C12(0)

Ag-Ag Ag Ag-Ag

2

Ag In Ag-In 1

### S

### (0)

### [ 1

### ρ C

### (0)

### ρ ρ C

### (0)

### ]

###

###

**4 **

**R**

**ESULTS**

The square well potential parameters of the
pure components are used for the study of Ag-In
melts at different compositions. The parameters
taken from literature 16_{ and are given in Table 1. }

A necessary condition in the application of Le-bowitz equations is s22>s11. Here s11 corresponds

to the diameter of Ag and s22 refers to the

diame-ter of In. The PSFs in long-wavelength-limit are obtained through eqns. (7) to (9) and are pre-Three partial structure factors (PSFs) in the

long-wavelength-limits can be written in terms of direct correlation functions C11(0), C22(0) and

C12(0)

Ag-Ag Ag Ag-Ag

2

Ag In Ag-In 1

In In-In

### S

### (0)

### [ 1

### ρ C

### (0)

### ρ ρ C

### (0)

### ]

### 1

### ρ C

### (0)

###

###

###

###

(7)### (0)

### C

### ρ

### 1

### (0)

### S

### (0))]

### C

### ρ

### [1

### (0)

### S

In -In In Ag -Ag Ag -Ag 1 In -In_{}

###

###

(8)### (0)

### C

### ρ

### 1

### (0)

### S

### (0)

### C

### )

### ρ

### ρ

### (

### (0)

### S

In -In In Ag -Ag In -Ag 2 1 In Ag In-Ag

###

_{}

(9) Thus for the binary alloy the total structure

factor can be written as

2 1 / 2

Ag Ag Ag-Ag Ag In 2 Ag In Ag-In In In In-In

2 2 1

Ag Ag In In

### S(0)

### [c f S

### (0)

### 2 (c c )

### f f S

### (0) c f S

### (0)]

### X [c f

### c f ]

###

###

###

###

(10) Here fAg and fIn are atomic scattering factors

and cAg and cIn are the atomic fractions of Ag

and In respectively.

Important relations also exist between Bhatia-Thornton (BT) correlation functions in the long wave length limit and Sxy(0) and also be 19

CC Ag In In Ag-Ag

Ag In-In 1 2 Ag In Ag-In

### S (0)

### c c [c S

### (0)

### c S

### (0)

### 2 (c c ) S

### (0)]

###

###

###

(11)

The CSRO can be obtained from SCC(0) as 8

CC CC

CC 1

1

CC 1

### S (0)

### S (0),id

### α

### S (0)

### S

### S

### S (0)

### S

###

###

###

###

###

###

###

(12) Here 2 1 CC### (0),

### id

### c

### c

### S

###

(13)and S1 is the deviation of the concentration –

concentration correlation function in the long wavelength limit from its ideal value,

###

is the coordination number can be computed from the total radial distribution function obtained from the Fourier transformation of the total structure factor S(k)##

###

###

min 0 2### dr

### r

### g(r)

### ρ

### π

### 4

*r*(14)

Further, DM and Did can be given by Darken

thermodynamic relation as 10

### (0)

### S

### C

### C

### D

### D

CC 2 1 idM

###

_{ (15) }

with 1 1 M 1 id

### C

### a

### 1

### D

### a

### D

###

###

###

(16)DM = C2D1 + C1D2 (17)

where D1 and D2 are the self-diffusion

coefficients of pure components and a1 is the

activity of first component, Ag in binary melts.

** (nm) **

**/kB **

**(Degree **
**Kelvin) **

Ag 0 .260 500.00 1.75

In 0 .283 173.86 1.70

sented in Table 2. The total structure factor in long-wavelength limit, S(0) was evaluated from equation (10) and are given in Table 2 and also presented as a function of concentration in Fig-ure 1. The DM values at different compositions

are calculated by Venkatesh et al. 16_{ and }

there-fore not repeated here but employed in the com-putation of Did at the same compositions.

Computed values of ψ, SCC(0), DM, Did and α

are listed in Table 3. Further, to understand the chemical ordering in the alloy, the ratio DM/Did

and α are plotted as function of concentration in Figure 2.

**D**

**ISCUSSION**

Unfortunately, there are no experimental values forpartial structure factors (PSFs) in the

long-wavelength limit and isothermal compressi-bility are available for comparison. Thus, it can be seen from Table 2 in the high composition region of Ag up to 50% Ag-Ag correlation in long-wavelength-limit is favourable whereas as In-In correlation is favourable at lower % of In. In high % of In cross correlation is favourable and this opinion can be supported by the ob-served SCC(0) values beyond 70% of In as

pre-sented in Table 2. Decrease in SCC(0) is an

indi-cation of compound formation between
compo-nents of the alloy 8_{. S(0) against % of In is }

plot-ted in Figure 1 it can be observed that this value also decreases between 35 to 40% of In and also beyond 70% of In.

Computed values of SCC(0) with their ideal

values, i.e SCCideal(0), total coordination number,

ψ and the CSRO, a at different atomic fraction

**% of In in **
**Ag-In alloy **

**Temperature **

**(K) ** **SAg-Ag(0) ** **SIn-In(0) ** **SAg-In(0) ** **S(0) **

20 1123 0.515 1.153 -0.743 0.033

30 1023 0.908 1.197 -1.015 0.035

40 873 1.569 1.314 -1.409 0.036

50 873 1.679 0.948 -1.231 0.039

70 873 1.425 0.367 -0.682 0.041

80 873 1.260 0.206 -0.459 0.041

90 873 1.118 0.103 -0.271 0.040

**% of In in **
**Ag-In alloy **

**Coordination **

**Number (Z) ** **SidCC(0) ** **Scc(0) **

**DM x 10-9**

**(m2 _{/s) }**

**Did x 10**

**-9**

**(m2 _{/s)}**

**α**

20 12.5 0.09 0.110 0.9 1.309 -0.04

30 11.8 0.16 0.243 0.9 0.778 0.013

40 11.9 0.21 0.450 0.8 0.427 0.043

50 11.6 0.25 0.407 0.8 0.491 0.035

70 11.2 0.24 0.154 0.8 1.091 -0.030

80 10.8 0.21 0.065 0.9 2.215 -0.11

90 10.5 0.16 0.016 0.9 5.063 -0.27

Table 2. Computed values of PSFs and total structure factor S(0) in long-wavelength-limit at different atomic % of In in Ag-In liquid alloys.

**6 **
of In in liquid Ag – In liquid binary alloys are

shown in Table 3. A liquid binary alloys can be classified on the basis of their concentration de-pendent SCC(0) data. If SCC(0) < SCCideal(0) for

those concentrations liquid metals components in binary melts show compound forming nature and exhibit some short range order while, SCC(0)

> SCCideal(0) at these concentrations components

show demixing tendency.

D12/Did approaches 1 for an ideal mixing and

less than 1 of this ratio shows phase separation and more than 1 indicates the compound forma-tion tendency in binary mixtures. From Table 2 we confirm that the computed results of SCC(0)

for 0.30 to 0.70 atomic fraction of In in Ag-In melts have higher values than their correspond-ing ideal values and this shows the segregation tendency of Ag and In atoms. This outcome is also supported by positive values of a and less than 1 values of D12/Did between this

concentra-tion range 10_{ as can be seen from Figure 2. The }

negative difference of SCC(0) from their

corre-sponding ideal values and the condition D12/Did

> 1 inform that there is complex formation

be-low 0.30 and above 0.70 atomic fractions of In. The CSRO parameter varies between –1 to 1, with negative values indicating the short range atomic ordering in the melt and positive values indicating segregation of atomic constituents.

**C**

**ONCLUSIONS**

Considered alloys show compound forming nature between 0.7 to 0.3 atomic fractions of In, hence, there must be some ordering potential between components of binary alloys. The per-turbation of hard sphere with square well inter-action is suitable model for such calculations. Microscopic functions of the alloy were deter-mined using potential parameters of pure com-ponents. There is no evidence for experimental results of SCC(0) from scattering properties of the

alloys, however, experimentalist determine this function by analyzing experimental thermody-namic activity data so the purposed model cal-culation is very useful for understanding the chemical ordering in binary melts.

Figure 1. % of In in Ag-In alloy vs S(0)

**R**

**EFERENCES**

1. Gopala Rao RV & Satpathy A (1990).
Statistical-mechanical model in the evaluation of partial and total
structure factors, atomic distribution functions, and
diffu-sion coefficients of silver-tin liquids at various
concentra-tions. *Phys Rev B*, **41**, 11938.

2. Anusionwu BC, & IIo-Okeke EO (2005). Segregation
and surface properties of In-Zn liquid alloys. *Phys Chem *
*Liq*, **43**, 25–36 .

3. Awe OE & Olawole O (2012). Correlation between bulk
and surface properties in Cd-X (X=Hg,Mg) liquid alloys. *J *

*Non-Cryst Sol,***358**, 1491–1496.

4. Singh NKP, Singh RN & Choudhary RB (1991).
Thermo-dynamic investigation of atomic order in AlMg liquid
alloys. J Phys Condens Matter, **3**, 3635.

5. Gonz’alez DJ, Gonz´alez LE, Opez JML & Stott MJ
(2005). Collective modes in liquid binary alloys. An ab
initio molecular dynamics study of the LiMg and LiBa
alloys. J Phys Condens Matter, **17**, 1429.

6. Mishra PP, Milanarunb M, Jha N & Mishra, AK (2002).
Thermodynamic properties of liquid glass-forming Ca–
Mg alloys.*J Alloys Compd,***340**, 108.

7. Odusote YA (2008). Investigation of ordering
phenome-non in Me-Pt (Me=Fe,Ni) liquid alloys. *Sci Technol Adv *
*Mater,***9**, 1–7.

8. Singh RN & Sommer F (1997). Segregation and
immisci-bility in liquid binary alloys. Rep Prog Phys, **60**, 57.
9. Khaeque MA, Bhuiyan GM, Sharmin S, Rashid RIMA &

Rahman SMM (2002). Calculation of partial structure
factors of a less-simple binary alloy. *European Phys J B,*

**26**, 319.

10. Singh BP, Adhikari D & Jha IS (2012). Short range order
in molten Al–Si alloys. *Phys Chem Liq,*50, 697.

11. Mendelev MI (1998). An iterative procedure for the
crea-tion of computer models of non-crystalline materials
from diffraction data. *J Non-Cryst Solids*,223, 230.

12. Mendelev MI (1998). Computer simulation of Ag–In
liquid alloys structure and self-diffusion coefficient
calcu-lations.*J Non-Cryst Solids*, **232**, 560.

13. Arai Y, Shirakawa Y, Tamaki S, Saito M & Waseda Y
(1998). Structural properties of liquid Ag-In system. *Phys *

*Chem Liq*,35, 253.

14. Kes H, Dalgic SS & Dalgic S (2005). Structure of less
simple liquid alloys: AgX-In1-X, *J Optoelectron Adv Materials*,

**7,** 2047–2057.

15. Bhuiyan GM, Ali I & Mujibur Rahman SM (2003).
Atomic transport properties of AgIn liquid binary alloys.
*Phys B: Condens Matter*, **334,** 147.

16. Venkatesh R, Mishra RK & Gopala Rao RV (2003).
Structural, thermodynamics and other associated
proper-ties of partially ordered Ag-In alloy. *PhysStat Sol B*, **240,**
549–560.

17. Lebowitz JL (1964). Exact solution of generalized
Percus-Yevick equation for a mixture of hard spheres. *Phys Rev,*

**133A**, 895.

18. Gopala Rao RV & Venkatesh R (1989). Computation of

total and partial structure factors, coordination number,
and compressibility with self- and mutual-diffusion
coeffi-cients of Hg-In alloy. *Phys RevB*,** 39**, 3563.